G. H. ~ a n ~ o land la~
Icium Phosphate on Hydroxyapatite Crystals. Effect of ~ u p e r ~ a t u r aand ~io~
Hi. Nancollas" and B. Tomaii6' Chemistry Department, State University of New York at Buffalo, Buffalo, New York 142 14 (Received April 3, 1974) ~ ~ ~ ~ cosb ~ i ~assisted ~ ~ t by i the o nNational institutes of Health
The kinetics of growth of hydroxyapatite seed crystals has been studied a t 25' and a t constant physiological pM in stable supersaturated solutions of calcium phosphate. The grown material was characterized chernically and by infrared and X-ray powder diffraction methods. The pH was maintained by means of the pH-Stat-controlled addition of base and the growth was followed by analyzing the solutions for calcium and phosphate. Experiments have been made over a wide range of initial supersaturation in order to obtain information about the nature of the calcium phosphate phases formed. The overall precipitation reaction involves not only the formation of different calcium phosphate phases but also the concomitant dissolution of the thermodynamically unstable phase octacalcium phosphate formed rapidly in the initial stages of the reaction. Dissolution of the solid material formed in the crystallization experiments indicated a stoichiometry corresponding to OCP. The results of growth experiments a t low supersaturation and in the presence of neutral electrolytes are discussed in relation to the calcium phosphate phases formed under these condition$;.
Introduction Although the precipitation of calcium phosphates and in particular hydroxyaipatite [CaS(PO&OH, hereafter HAP] has been extensively studied, there remains considerable uncertainty as8to the nature of the phases formed during the early stages of the precipitation r e a c t i ~ n . ~The - ~ eventual transformation of these phases into the thermodynamically stable NAP phase is also little understood. Since the process of H I P formation is very slow, thermodynamic data such as solubili.ties are not readily accessible since the attainment of true equilibrium is not easily ensured. A major difficulty is that different workers have used very different experimental methods both in the preparation of the calcium phosphate phases and in studying the course of the precipitation reactions. Thus crystalline materials prepared under conditions of high temperature are sometimes studied in aqueous systems at room temperatures and behave quite differently from the calcium phosphates prepared a t ambient temperatures. It will be apparent from the results of the present work that the nature of the iniphases and the course of the subsequent crystal growth reaction is markedly dependent not only upon the degree of supersaturation of the solution, but also on the ionic strength of the solution and the type of neutral or inert electrolyte present. The wide range of conditions used by other workers makes it very difficult to compare their results and this has contributed a great deal to the present unsatisfactory state of knowledge. 'l'ho solubility product, Ksp, of well-defined crystalline HAP has been. ~ ~ e t e ~ m ~from n e dthe results of dissolution experiments but the ported values of K,, range from 10-556 to 101eio.7 The ssolution of HAP is a moderately fast process arid, as an example of a weathering reaction, the congruent dissolution is probably straightforward. Many published data., however, reveal that in the process of HAP crystal growth, equilibrium conditions cannot be attained, in e x p e ~ i m ~ nreasonable ~ ~ ~ ~ l y times.s For this reason, analysis of solid-solution experimental data solely on the The Journal o! P h w c a l Chemistry. Vol, 78. No. 22, 1974
basis of thermodynamic solubility products is an oversimplification. Kinetic considerations may -be of paramount importance in controlling the formation of the calcium phosphate phases during the Precipitation reactions. Thus in the case of calcium phosphate precipitation at physiological pH, the initial rapidly formed amorphous precursor undergoes a slow transformation to AP and significant changes, with time, are observed in such factors as chemical composition, the degree of ~rystallinity,~ and the specific surface arealo of the solid phases. The spontaneous precipitation of calcium phosphate from its supersaturated solutions has been extensively studied. The critical precipitation point is usually determined by the slow mixing of solutions containing calcium and phosphate ions and observing the first appearance of solid phase. This procedure suffers from the disadvantage that a considerable amount of precipitatio~has already taken place before the precipitate is visible in the solution. The usual assumption of homogeneous nucleation is also open to question since it is doubtful if any medium i s sufficiently free from foreign nucleating sites to preclude the possibility of heterogeneous nucleation. For these reasons, it is very difficult to reproduce the resdts of spontaneous nucleation experiments and the present work is concerned with the growth of well-defined seed materials persaturated solutions of calcium p ~ ~ s ~ h a t e . ments have been shown to be highly r ~ p r o d ~ c ~ b ~ eand ~l,12 studies can be made of the effects of factors such as the level of supersaturation, seed morphology, and the presence of foreign ions. Thus logical level a t which d (hereafter DCPD) is the s that crystal growth of seed crystals from stable supersaturated solutions, under conditions of both variable and constant pH, is controlled by a surface reaclion a t the crystalsolution interface. The rate of crystal growth is proportional to the square of the supersaturation and is independent of the fluid dynamics within the system.13 congruent dissolution of DCPD crystal9 into subsaturated
Growth of Calcium Phosphate on HydroxyapatiteCrystals
solutions is diffusion controlled and the rate is directly proportional to the degree of ~ndersaturati0n.l~ The present work i s concerned with the growth of HAP seed crystals under conditions of physiological pH. This system is considerably more complex than that for DCPD '\and the simple kinetic equation which applies in the latter can no longer be wed. Factors such as solid surface:solution ratio, level of supersaturation, and the presence of neutral electrcrlyte have been studied in order to throw more light on the precipitation of calcium phosphates under physiiological conditions.
Materials Reagent grade materials were used in all experiments. Weli-crystallized HAP seed material was prepared by the method of Nancollas and Mohan.8 Crystal Growth Experiments. The crystal growth experiments were performed in a water-thermostated doublewalled vessel using stable supersaturated solutions of known supersaturation. The solution was stirred with a magnetic stirrer at about 250 rpm, and nitrogen gas was bubbled throughobt the experiment to exclude carbon dioxide. The pH was measured with a glass electrode-calome1 electrode pair connected to the Metrohm Herisau pHStat (Model Combit itrator 3D). The electrode systems were standardized before and after each experiment with NBS standard buffer solutions prepared according to Bates:15 0.025 iM potassium dihydrogen phosphate 0.025 M disodium hydrogen phosphate, pH 6.865 and 0.01 M borax, pH 9.180 at 25'. Calcium chloride and phosphoric acid solutions were mixed at the desired molar ratio (1.66 unless otherwise stated), and the pH was adjusted to 7.40 f 0.01 by the pH Stat addition of 0,05 M base. Following the addition of a known amount of seed slurry, crystal growth was monitored by pH-Stat addition of 0.05 M alkali metal hydroxide. A t E,nown times, samples of solution were withdrawn from ',he ceil and filtered through Millipore Celotate filters of 0.22-p pore size. The solution phase was analyzed for total calcium and phosphate. Calcium solution concentration was determined by atomic absorption spectroscopy, using a 303M Perkia -Elmer spectrophotometer; a typical calibration line had the following parameters: [Ca] X lo-* ( M ) =: (5.37 f hi.O7I(absorbance) - (0.0236 f 0.008), with the standard deviation of determination of 0.02 ppm in the range of 1-8 ppm Ca. Phosphate solution concentration was determined spectrophotometrically by the phosphomolybdate m e t l l ~ a d A . ~typical ~ calibration line had the fol(1M)= (4.928 k 0.119)(ablowing parameters. [I)] X sorbance) - (0.214 It 0.093); the standard deviation of determination in ihe 10 -- 50 M Mrange was 0.5 pA4. The solid phases after lyophilization were further characterized bl7 X-ray diffraction, infrared spectroscopy (Nujol mulling technique and KBr-pellet method), and dissolution experiments. The X-ray diffraction (Cu K a radiation) examination of seed material and grown products was performed usin,g a Philips XRG-300 X-ray diffractometer coupled to a recorder. The relative crystallinity of grown samples was estimated semiquantitatively from. a linear regression line using known crystalline and amorphous synthetics as standards, measuring the intensity of the unre~ calcium phosphate was solved 211 r e f l e c t i o ~ lAmorphous prepared by sponl ous precipitation from calcium phosM pyrophate solutions at 7.40 in the presence of phosphate as described by Francis.ls Mixtures with HAP were prepared by weight (50 mg total) and carefully ho-
mogenized in an agate mortar with 1 drop of mineral oil. The resulting paste was evenly spread on a glass plate in order to avoid the preferential orientation of crystallites, as would be the case if pellets were used. The relative intensities of the 211, 112, and 300 reflections were 100,60, and 60 as given for mineral hydroxyapatite.19 The standard deviation of determination was 2.67%.
Results and Discussion It is first necessary to express the degree of supersaturation in the stable supersaturated solutions with respect to the various possible calcium phosphate phases, DCPD, octacalcium phosphate (Ca4H(P04)3, hereafter written OCP), tricalcium phosphate (Ca3(PQ&, hereafter TCP), and HAP. In addition to the concentration of calcium and phosphate ions in the solution, the supersaturation depends upon the pH, temperature, and the concentration of other "neutral" electrolytes. The degree of supersaturation with respect to each of the calcium phosphate phases can be expressed in terms of the appropriate ionic concentration products (Scap,eq I), the calculated free calcium ionic SCaP
IP - K,, ? i -
concentration (Sea, eq 2), or the Gibbs free energy of trans-
[ ~ a ~ '] , [ca"], [ca2+],
fer from supersaturated to saturated solution (AG, eq 3). IP
IP A G = -RT In(3 ) KSD corresponds to the activity product in the supersaturated solution defined, for each calcium phosphate phase, by eq 4-7 where K,, is the value of IP at equilibrium (Ksp IP,,,,
( I C ~ * + ] ~ ~ ) ~ ( [ P O/ ~[H+]J,~ - I J(7) ~)~K~
(DCPD) = 2.1 X 10-7,20 K,, (OCP) = 1.25 x 10-47,21K,, (TCP) = 1.15 X 10-29,22and K,, (HAP) = 1.8 X 10-58,23), [Ca2+]t is the free ionic calcium Concentration at time t and [Ca2+], is its equilibrium value, and -AG represents the affinity of the reaction.24 Concentrations of the ionic species in the solutions were calculated as described prev i o u ~ l yfrom ~ ~ mass balance, ellectroneutrality, proton dissociation, and calcium phosphate ion-pair association constants12 by successive approximations for the ionic strength, 1. The activity coefficients of 2-valent ionic species, fz, were calculated from the extended form of the Debye-Huckel equation proposed by Davies,26 -log fi = Az2(1112/(1 11/2) - 0.3 I ) . Growth Experiments of High Supersaturation. In most of the previous spontaneous precipitation work, relatively high concentrations were used and the solutions were considerably supersaturated with respect to all of the calcium phosphate phases. These conditions are, however, far removed from those in uiuo. In the present work, experiments made over a range of supersaturation are summarized in
The Journalof Physical Chemistry, Vol. 78, No. 22, 7974
6 ,H. ~ a ~ c oand ~ lB.a Tomalit ~
TABLE I: Coricentration and Supersaturation D a t a of Some Typical Calcium Phosphate S u p ~ ~ ~ ~ t u r a t e ~ Solutions Prior to Inoculation (pH 7.40,25 ")
no. type ________-__
Total Total /calcium 1, [phosphate 1, mM mM
Ionic strength, mM
TABLE 11: Callciumt Phosphate Crystallization Induced by the Addition of HAP Seed (0.2 g of Seed L-') a t 25O, pH 7.4 Initial Initial concn rate, - AT,,/ 1.03!rp, Neutral At, p M Expt 103rrClr, IM M electrolyte min-1 g-1 Base no.
- AG [NaCI 1, mM
Phase DCPD OCP TCP HAP DCPD OCP TCP HAP DCPD QCP TCP HAP
0.66 1.60 1.17 1.23 -0.78 -0.87 5.95 3.29 -0.44 2.21 6.82 1.26
(es 3), (eq 2) kcal mol-' 0.24 0.27 2.96 1.1 4.19 3.4 43.6 15.07 ---0.56 -0.91 .-0.33 -1.16 0.53 1.22 12.5 10.27 -0.12 -0.37 0.71 0.18 2.52 1. .30 18.0 12.45 SCa
X IO2 X lo3 X 10"
X PO7 X 10
x 109 ,,,'
mM C a
46 77 84 72 71 73 74 79 76 28 29 27 26 25 24 23 10
21 25 13 19
1.477 0.934 0.709
0.677 0.501 0.4511 0 .432
0.374 1.611 1.616 1 .ti20 1.583 1.576 1.670 1.616 1.609 1.601 1.576 1.565 1.672
1.041 0.617 0.449 0.377 0.340 0.301 0 ,287
0.247 0.987 0.979 0.96'7 0,970 0.987 0.972 0.97'7 3. ,013 0.921 0.987 0.968 0.955
420 200 112 60 48 57 40 48 43 550 0.01 M NaCl 315 0.05 M NaCl 192 0.10 NaCl 195 0.15 NaCl 165 0.40 NaCl 77 0.70 NaCl 77 0.15 M LiCl 193 0.15 M NHdC1 190 0 . 1 5 M N a C l 165 0.15 M KCl 118 0.15MCsCl 65
KOH KOH KOH KOH KOH KOH KOH KOH KOH NaOH NaOH NaOH NaOH NaOH NaOH NaOH LiOH NHdOH NaOH KOH CsOH
Tables I and Ik Negative values of Sea, and -AG represent undersatmaticln with respect to the particular phase considered. In systems I1 and I11 it was possible to control the driving force to avoid the formation of some of the calcium phosphate phases. HAP is the least soluble phase at pH 7.40 and, in the absence of kinetic complications, it should be the thermodynamically most stable.27 The results of a typicill experiment (expt 46) a t relatively high supersaturation iire shown in Figure 1 in which the concentration of calcium io11 is plotted as a function of time following the addition cf 200 mg of HAP seed crystals to the stable supersaturated solution. On the basis of the calculated concentrations of the calcium and phosphate ions, the ionic products of each of the calcium phosphate phases corresponding ]toequilibrium are also included in Figure 1. It can be seen i n Figure 2 in which the driving force, -AG, is plotted agairwt time that the solution became undersaturated with resl~ectto DCPD after a relatively short time (approximately 10 min) while supersaturations of OCP and TCP were maintained for about 40 and 570 min, respectively. At all states of the reaction the solution was highly supersaturated with respect to HAP. The Journal of Physical Chemisfry, Vol. 78, No. 22, 1974
TIME ( m i n )
Figure 1. Crystal growth at high supersaturation. Plots of total calci-
um concentration (full line) and base uptake (dotted curve) as a function of time for expt 46.
In Figure 1, it can be seen that immediately following inoculation with seed crystals, the very fast growth commences. The initial rate of reaction normalized for seed or solid-phase concentration was estimated to be -ATCa/At = 420 p M min-l g-l. After about 30 min, the rate decreased (-ATCa/At = 5.3 pM min-l g-l), until almost zero a t 200 min following which there is a further increase from 3 to 8 hr characterized by a rate of growth of about 2.5 bh4 min-l g-l. This discontinuity in the rate curve is paralleled both in the soluble phosphate level and in the potassium hydroxide uptake required to maintain tbs p interesting to note that the break in the growth curve a t 200 min was not noticeable in previous works in which considerably less seed material was employed. The presently studied high so1id:solution ratio is certainly of considerable importance since in physiological systems such as the boneserum interface the mineral surface area3 involved are very large. The observed inflection in the growth curve probably arises through the superposition of a number of kinetic processes which take place a t different rates and provides further evidence for the involvement of more than one calcium phosphate phase in the precipitation of HAP. The results may be expressed in terms of the molar ratios of calcium to phosphate A[Ca]/A[P], which har7e precipitated at any instant. The data are given in Table I1 where A[Ca] = Tc,(initial) - Tc,(time t ) and A[P] -- T,(initial) T,(time t ) , T c a and T , being the total concentrations of calcium and phosphate, respectively; the uncertainty in A[Ca]/A[P] is about f0.05 or less. It can be seen in Table I11 that A[Ca]/A[P] decreases from relatively high values during the first 20 min of reaction to the value of 1.45
Growth of Calcium ~ h ~ s OR~ Hydroxyapatite ~ ~ a ~ e Crystals
TABLE 111: Cryetd G r o w t h of Calcium Phosphate on Crystalline HAP Seed (High Supersaturation) a Amt of 0.55 M
t, min MOH, ml
1o3[Ca], 103[P1, A[Ca]/ M M AfPl
3. ,562 1.208 0.996 0.812 0.738
95 150 180 210 240 300 360 420
5 10 20
0.973 0.764 0.621 0.477 0.408 0.357 0.316 0.281 0.284 0.282 0.270 0.232 0.209 0,197 0.187 0315 0,894
1.72 1.61 1.51 1.46 1.44 1.45
1.45 1.48 1.48 1.47
89 86 80 68 77
1.48 1.50 550 0.368 1.52 1200 0.202 1.52 1440 0.186 1.56 a Table I, syrsteni I ; 0.2 g of speed crystals I.-'; initfa1volume; pM 7,43,25"; expt 46 and 47. 0.427 5.396
% cryst (HAP)
which remains quite constant up to about 300 min. This value was also found in previous experiments in which a considerably smaller amount of seed material was used.8 At longer times, the ratio gra ually increases but the value of 1.67 nequired fo? HAP stoichiometry was not reached even after 3 days of reaction at 25'. It is doubtful if these A[Ca]/ ALP] values are useful indicators of the types of calcium phosphate phams formed since, as will be seenglater, the overall precipitstion reaction under the conditions of these experiments m,iy involve not only the formation of different calcium phosphate phases but also the concomitant unstable phase formed dissolution o f a thern~odynam~cally rapidly in the initial stages of the reaction. In order t o gain more information about the nature of the cslcium phosphate phases, X-ray powder diffraction and infrared ~ ~ ~ e s t ~ g a twere i Q nmade s on the solid phases formed a t each stage of the precipitation reaction. In Figure 3 X-ray data are shown for the solid phase taken from the crystal1i:zal;inn cell a t 60 min of reaction (expt 47), taking the precautions described to avoid preferential orientation of the cryttallites. It can be seen that the positions of the peaks are identical with those of the HAP seed crystals and i n none of the experiments was any X-ray evidence found for the existence of other calcium phosphate phases. The particles ai' suck phases, if formed, were therefore too all to be cletixted by the X-ray diffraction method. Thus wii and coworkerszs have stated that lamellar mixtures of OCP and H4P are undistinguishable when the crystallites are as thin 9s 25--75 A,Assuming that the grown material consists of a mixture of crystalline HAP and polymorphic forms which have the same mass absorption coefficients, the p e r c ~ ~ icrystallinity t a ~ ~ ~ was calculated using the method of K lug and Alexander17 on the basis of 100%crystallinity of the original HAP seed material. The data are presented in Table [III which shows that the percentage crystallinity decreases for the first -200 min following the addition of the seed crystals but thereafter increases. In the early &ages of growth, the peak width increases which indicates a decreasie ~ n naverage particle size, most probably due to the formstticin of amorphous or microcrystalline precursors. At later reaction times, the peak width gradually decreases again, iidicating an improvement of crystallinity of
grown product. This is in general agreement with observations made on spontaneously precipitated [email protected]
These results suggest that a t the very early stages of HAP seeded growth, an amorphous phase is formed which subsequently undergoes conversion to Crystalline material with an apatitic X-ray pattern. Eanes and PosnerZ9have studied the spontaneous precipitation reaction and found that the rate of conversion into the crystalline phase was proportonal to the amount of the crystalline phase present; the estimated particle size was -115 8, which is considerably smaller than in the present work. The conversion of amorphous to crystalline phase may involve an epitaxial matching of the depositing phase onto the HAP crystalline substrate and this explanation is quite consistent with the suggested autocatalytic conversion m e c h a n i ~ m .Because ~,~~ of the similarities between the structures of Od' HAPzs epitaxial overgrowths of these phases will easily occur. It will be particularly likely in systems such as those of the present work where rapid variation in the eomposition of the liquid phase occurs in the immediate vicinity of the growing crystal. The hydrolysis of QGP crystals to pseudomorphs whose properties progressively approach those of HAP takes place rapidly a t temperatures above 50°.28At 25', the hydrolysis reaction will be expected to be slow compared with the formation of the amorphous calcium phosphate phase. The infrared spectra of calcium phosphate phases have been described by Fowler, Moreno, and Brown.30 In many cases, the 3570-cm-1 OH stretch absorption anticipated for HAP is very weak. A possible explanation for such an effect i s that some portion of the QH groups are not detected because of the poor resolution associated with the small size of crystallites of high strain content. On the 0th growing material may be deficient in O H since the growth product a t the early stages. Consequently, the relative intensity of the particular band may be decreasing. However, neither the HAP seed nor any of the grown solids exhibited any absorption in the 1400-150O-cm-~ range characteristic of the presence of carbonate. This rules out the possibility of OH--CQ32- substitution and demonstrates the effectiveness of the measures taken to exclude carbon dioxide from the system. Fowler, Moreno, and Brown3" and Termine and Eanes31 have suggested that the bands at 865 and 910 cm-l, characteristic of OCP, may be useful for identifying OCP in the presence of MAP. In our grown materials the 910-cm-l band was completely absent but there was a diffuse absorption peak a t 865 cm-' indicating the presence of some OCP in the samples grown a t higher supersaturation (Table I, system I). Dissolution Experiments. The data presented above (eg., Figure 1)strongly suggest that the precipitation of calcium phosphate onto crystalline HAP seed crystals is made up of a number of parallel processes. Under the conditions of higher supersaturation it is clear (Figure 2) that the formation of up to four different calcium phosphate phases is possible in the very early stages of the reaction. The A[Ca]/ A[P] ratio during the first several hours of growth (-1.45) is very close to the ratio for the freshly precipitated "amorphous" calcium p h ~ s p h a t e .In ~ order to obtain further chemical information about the nature of the early developing phases, a number of dissolution experiments have been made under conditions of controlled pH. A 50-ml sample of calcium phosphate slurry was withdrawn from the crystallization cell a t a known time and quickly filtered, and the solid 10-12 mg was transferred to another cell conThe Journal of Physical Chemistry, Vol. 78, No. 22, 1974
@. H. Nancollas and E. Tomafit
TABLE IV: Comparison of Precipitation and Dissolution Data (Expt 77)
Crystal growth 10
- ,A G
K co l h
Time of Material sample 103[Ca] deposwithdeposited, drawal, ited, A[Ca]/' min M A[PI
30 70 140 240 300 360
0.764 0.858 0.947 0.976 1.046 1.088 1.331
1.49 1.48 1.49 1.50
103[Ca] after 60 min of
D is[Ca]. solved after 60 [Call [PI min of after dissoln 60 min
44 32 28
30 I9 17
1.33 1.33 1.38 1.37 1.32 1.33 1.57
[Ca] dissolved, expressed as per cent of Ca deposited (column 2).
100 1000 T I M E (min) Figure 2. Plot of the driving force (-AG)against time for expt 46: 0, total calcium concentralion (right-hand ordinate): 0 ,HAP; A, TCP: 0 ,OCP; v,DCPC) (left-hand ordinate).
H A P SEEDED G R O W T H
7 ' I 7
Figure 4. Growth at high supersaturation, plot of total calcium, 0, and ACa/AP, A,as a function of time (expt. 77). Dissolution experiment: A 7Ca/P in solution after 60 min: @, TCa value after 60 min, at the given time. dissolution of sample taken from growth run (0) 10
Figure 3. X-Ray powder lpatterns (Cu Kcu radiation) for expt 47.
taining 50 ml of a soldium chloride solution (6 X 10-3 M ) having an ionic strength close to that in the growth cell. The pH was maintained a t a value of 7.40 by means of the pH-Stat-controlled addition of 5 X M hydrochloric acid solution. Ilissolution, which proceeded relatively rapidly, was followed for a period of 60 min a t the end of which time the soiid phases were separated and the solutions analyzed for calcium and phosphate. In Table IV and Figure 4, the molar ratios of calcium to phosphate dissolved from the grown solids after 60 min are compared with the corresponding A[Ca]/A[P] growth molar ratios a t the given time intervals. The calculated thermodynamic ionic products a t the end of the 60-min dissolution period show that the resulting solutions were undersaturated with respect $0 DCPD, OCP, and TCP but supersaturated in H,4P. If the dissolution reaction is allowed to proceed, after some I20 min, the pH begins to fall and a precipitation reaction takes place. However, since the composition of the solution remains undersaturated with respect to DCPD, OCP, and TCP, it follows that if these phases are present, their dissolution generates calcium and phosphate fur the formation of the least soluble phase, HAP. It is interesting t o note (Table IV) that the stoichiThe Journal of Physical Chemistry, Vol. 78, No. 22, 1974
ometry of the dissolving phase indicates that OCP may be one of the unstable precursor phases. This is in agreement with experimental evidence that OCP is formed as the first precipitation product in the process of spontaneous precipi t a t i ~ n .The ~ ~ ,relative ~~ amount of the precipitated phase which dissolves with OCP stoichiometry (Table ZV, column 5 ) decreased with time. It is significant that the corresponding dissolution [Ca]/[P] ratio for later stages of the growth process (1200 min, Table IV) is considerably larger (1.57). This indicates that by that time, OCP or DCPD were no longer available for dissolution from the surface of the grown material, having already been dissolved in the composite growth process a t earlier reaction times. Therefore, the anticipated dissolution of TCP and/or HAP would lead to the observed higher dissolution [Ga]/[P] ratio. Growth Expwinzents at Low Supersaturation. I t i s clear from the above, as has been repeatedly stressed by Brown, Moreno, and other^,^,^,^^ that in studying the precipitation of calcium phosphate it is important to control the concentrations so that the degree of supersaturation of the solution with respect to the various calcium phosphate phases is defined. Frequently, the results of experiments over a wide range of supersaturations are compared with the expectation that the same calcium phosphate phases will be formed. Recently, Robertson33 has emphasized the importance of considering the concentrations of calcium and
hosphate on Hydroxyapatite Crystals TABLE V: Crgstal Growth of Calcium Phosphate on Seed (Low Supersaturation)“
0 10 60 200
0.79 1.07 1.13 1 34 1 ‘70 1 84. 2.00 2 11 2 20
360 660 1440 2040 2880 4440 6240
0.432 0.351 0.312 0.279 0.254 0.216 0.161 0.149 0.1132 0.120 0.115
0.287 0.245 0.218 0.199 0.183 0,160 0.120 0.115 0.106 0.102 0.097
1.94 1.76 1.74 1.73 1.71 1.65 1.66 1.67 1.69 1.67
Table I, system 11; 0.2 g of seed crystals l.-’; initial volume; pll 7.40, 25’; expt 79. a
m M Cs 1.0
300 400 T I M E (min)
Figure 6. Crystal growth of calcium phosphate in the presence of sodium chloride. Plots of total calcium concentration as a function of time: 4,no NaCI; V. 0.01 MNaCI: 0, 0.05 MNaCI; 0,0.15 MNaCI; A, 0.4 MNaCI; e, 0.7 MNaCI.
Figure 5. Seeded growth experiments at low supersaturation. Plot of calcium concentration against time under conditions of high supersaturation (curve a, 8). Each experiment at low supersaturation (curves b-f, e) ccammenced at a concentration given by the points of intersection of the curves with curve a. Curves b, d, and f are plots of total calciiirn Concentration against time for the first 60 min in each case and curve c was continued for 100 min.
phosphate ions in studies of heterogeneous nucleation by crystals of HAP. These experiments were performed in a medium which was still supersaturated with respect to BCP. Therefore his results indicating QCP as the unstable precursor in the induced growth are not surprising and agree with the rcadts of the present study. The results, ol: growth experiments made in solutions of low supersaturation (Table I, system 11, undersaturated in DCPD and OCP and supersaturated with respect to T C P and NAP) are shown in Figure 5 and a typical experiment is summarized in Table V. In Figure 5 , curve a (open circles) shows the crystal growth at high supersaturation (system I, Table I). s“,urvesm b-f (Figure 5) (solid circles) refer to experiments a t low initial supersaturation represented by their intersection with curve a. Thus growth curve f (and Table V) refers to an experiment in which HAP seed crystals were used t o inoculate a solution metastable with respect to TCP arid HAP (initial Tca = 4.32 X 1Q-4M and T p --- 2.87 X M pPI 7.40). Crystal growth commences immediately following the addition of seed and the initial rate was estimated as -A[Ca]/At = 48 pA4 min-l g-l. The A[Ca]/A[P] ratios during the €irst 100 min for points selected from Figure 5 have an average value of 1.76 with a standard deviation of 0.1 This is considerably higher than the value required for AI’ indicating the formation of a phase
rich in calcium. This contrasts the suggestion of Bell and coworkers34 that the surface of HAP has a tendency for preferential interaction with phosphate rather than calcium. The data in Table V show that the A[Ca]/A[P] approaches a constant value of 1.66 after several hours of growth indicating the formation of HAP. Clearly, under these conditions of low supersaturation, the calcium phosphates with lower calcium phosphate molar ratios, DCPD, OCP, and TCP, cannot form. Their subsequent dissolution does not, therefore, contribute to the overall A[Ca]/A[P] values. Striking confirmation of this suggestion was provided by the results of dissolution experiments made, as described above, at a constant pW and ionic strength. The product isolated after 4 days of growth under conditions of low supersaturation, dissolved a t a calcium:phosphate molar ratio of 1.69. The dissolution of HAP seed material resulted in a dissolution ratio of 1.72 and both values indicate that the growii material is HAP which undergoes congruent dissolution. The slightly elevated molar ratio as compared with the theoretical value of 1.67 may be attributed to surface phenomena and the presence of minor impurities as suggested by Avnimelech and
other^.^ Seeded Growth in the Presence of Neutral Electrolytes. In the normal crystallization runs, the pzI of the supersaturated solution was maintained by the addition of 0.05 M KOH. The results of a series of experiments made using similar concentrations of LiQH, NaOH, CsQH, and NH4OH showed that the kinetic rate curves had the typical shape shown in Figure 1 with the characteristic inflection of about 200 min of growth irrespective of which base was used. The effect of adding “neubal” electrolyte t o the system is, however, marked and the results of crystallization experiments in the presence of different concentrations of sodium chloride are shown in Figure 6. A study by Bell and his coworkers34 has shown that the point of zero change (PZC) of HAP suspensions is dependent upon the composition of the ionic medium. Although the PZC of the amorphous calcium phosphate precursor is not known, it is also likely that it will be dependent upon both the nature of the supporting medium and the history of the sample formation. The added electrolyte may therefore induce coagulation of the particles in a manner analogous to the classical colloid coagulation observed in so many systerns~a5Another influence of the added electrolyte is to decrease the effective supersaturation by reducing the activity coefficients of The Journal of Physical Chemistry, Vol. 70, N o . 22, 1974
IO0 1000 TIME (min)
Figure 7. Crystal growth in the presence of 0.15 M potassium (A), cesium (O), and sodium (D) chlorides. Plots of per cent of total calcium concentration againrjt time.
the lattice ion:? In the solution. This is clearly illustrated in Table 1 (system 111).It can be seen in Figure 6 that the addition of sodium chlioride markedly decreases the rate of crystallization and it IS interesting to note that the discontinuity characteristic of the high-supersaturation experiments (Figure 1) is absent. This result is consistent with the proposal that the sodium chloride simply reduces the driving force for reaction since a t an ionic strength of 0.15 M, DCPD and OCP do not form. It is the concomitant dissolutron of such phases in the early stages of reaction which appears to account for the observed inflection in the growth curves. Crystal growth experiments were made in 0.15 M lithium, potassium, cesium, and ammonium chlorides. The data for potassium, cesium, and sodium chlorides are presented in Figure 7. It can be seen that there is a marked effect on changing the nature of the alkali metal cation. Toward the end of the reaction (LOO0 min) the extent of crystal growth increases in the order. KCl < CsCl < NH&l < LiCl < NaCl. The greatest differences are found between potassium and sodium chlorides whach are of particular importance in biological systems. After 1000 min of growth 60% of the calcium is precipitated in the sodium chloride system whereas only 40% has deposited in the presence of potassium chloride. After 24 hr of reaction, A[Ca]/A[P] values are 1.45 and 1.61 for NaCL 2nd KCI, respectively. The precipitated solids a t these extended times contained from 5.5 to 6.0 mol % of sodium in tl-ir presence of sodium chloride but almost no potassium in the presence of potassium chloride. These results are an gocad agrrement with those of Newman and coworkers,36 vihci found khat sodium can replace calcium in the calcium phosphate solid whereas potassium is revers~ 2,urface. ibly adsorbed o r the Bell and r o w o r k e r ~have ~ ~ shown that the point of zero change of HAP occiirs at pH ‘7.5 in the presence of sodium chloride and at p 8.4 i n potassium chloride systems. In the present experiments, a t pH 7.40 an HAP surface would be appreciahly positively charged in the potassium chloride solution leading to a lower rate of crystallization. Unfortunately, no dectrokiinetic data are yet available for the “amorphous” r-alcium phosphate phase for which, being more colloidal, differme factors may be of importance. It is interesting 1 o note 1 hat X-ray powder patterns of solids grown in the prrsenct: of 0.15 M sodium or potassium chloside for 120, 240, 06 1440 min show no change from that of the EIitP seed ~ y s t a This l ~ ~indicates that the formation of the “amorphoiis” precursor is undetectable under these The Journal of FJhy>:icalChomisfry, Vol. 78,No. 22, 1974
Nancollas and 9.Toma%
conditions in contrast to the results a t an effectively higher supersaturation. This finding is in agreement with the results of the growth experiments made at low supersaturation. It is clear from the results of the present work that the concentrations of lattice ions in supersaturated solutions of calcium phosphate are very important in determining the nature of the calcium phosphate phase which separates on the addition of HAP seed crystals. Indeed, the type of phase formed may be influenced by careful control of the physicochemical conditions. This finding may be important in understanding mineralization in biological systems for which the supersaturation is low and the solidxolution ratio is very appreciable. The matrix of young bone contains a major proportion of an amorphous inorganic comp ~ n e n whose t ~ ~ formation is frequently attributed to the presence of a variety of potential crystal growth inhibitors in the body fluids. Unfortunately studies of model systems are usually made in media of very high supersaturation in order to provide appreciable measurable concentration changes. In the light of the present results, the reaction path may be markedly altered under such conditions. The use of low concentration levels is certainly more tedious and experimentally demanding but such studies may be closer to those in real biological systems.
Achnowledgment. We thank the National Institute of Dental Research for a grant (DE03223) in support of this work. References and Notes (1) On leave of absence from Rudjer Boskovic institute, Zagreb, Yugosiavia. (2)(a) M. D. Francis, Ann. N. Y. Acad. Sci., 131,694 (1965);(b) H. M. Rootare, V. R. Deitz, and F. Carpenter, J. Colloid Sci., 17, 179 (1962). (3)W. F. Newman and M. W. Newman, Chem. Rev., 53, 1 (1953). (4)E. D. Eanes, I. H. Gillessen, and A. S.Posner, Nature (London),298, 365
(1965). ( 5 ) W. E. Brown, Clin. Qrthop., 44, 5318 (1966). (6) E. C. Moreno, T. M. Gregory, and W. E. Brown, J. Res. Nat Bur, Stand., Sect. A, 72,773 (1968). (7) Y. Avnimelech, E. C. Moreno, and W. E. Brown, J. Res. Nat Bur..Siand., Sect. A, 77, 149 (1973). (8) G. H. Nancoilas and M. S. Mohan, Arch. QralBioi., 15, 734 (1970). (9)A. L. Boskey and A. S. Posner, J. Phys. Gbem., 77,2313 (1973). (IO)J. M. Holmes and R. A. Beebe, Caicif. Tissue Res., 7,163 (1971). (11)G. H. Nancollas and N. Purdie, Quart. Rev., Ghem. Soc., 18, l(1964). (12)~ R W. . Marshall and G. H. Nancollas, J. Phys. Chem., 73,3838 (1969). (13)G. H. Nancollas and J. S.Wefel, J. CrystalGrowtb, in press. (14)G. H. Nancollas and R. W. Marshall, J. Dent. Res., 50, 1268 (1971). (15)R. G. Bates, “Determination of pH,” Wiley, New York, N. Y., 1963. (16) D. N. Fogg and N. T. Wilkinson, Ana/yst (London),83,403 (1958). (17)H. P. Klug and L. E. Alexander, ,“X-Ray Diffraction Procedures,” Wiley, New York, N. Y., 1962. (18)M. D. Francis, Calcif. Tissue Res., 3, 151 (1969) (19)Powder Diffraction File No. 9-432,Joint Committee of Powder Diffraction Standards, Philadelphia, Pa., 1967. (20)E. C. Moreno, T. M. Gregory, and W. E. Brown, S. Res. Naf. Bur. Stand., Sect. A, 70, 545 (1966). (21)E. C. Moreno, W. E. Brown, and G. Osborn, SoilSci. Soc.Amer., 24,99 (1960). (22)E. C. Moreno in “Structural Properties of Hydroxyapatite and Related Compounds,” W. E. Brown and R. A. Young, Ed., Gordon and Breach, New York, N. Y.. Chapter 14,in press. (23)J. S.Clark, Can. J. Chem., 33, 1696 (1955). (24)W. Stumm and J. J. Morgan, “Aquatic Chemistry,” Wiley-lnterscience, New York, N. Y., 1970. (25)G. H. Nancollas, “Interactions in Electrolyte Solutions,” Elsevier, Amsterdam, 1966. (26)C. W. Davies, “Ion Association,” Butterworths, London, 1962. (27)W. E. Brown in “Environmental Phosphorus Handbook,” E. J. Griffith, A. Beeton, J. M. Spencer, and D. T. Mitchell, Ed., Wiley, New York, N. Y.,
1973. (28)W. E. Brown, J. P. Smith, J. R. Lehr. and A. W. Frazier, Nature(London), 196, 1048 (1962). (29)E. D. Eanes and A. S.Posner. Trans. N. Y. Acadl Sci., 28, 233 (1965). (30)8. 0.Fowler, E. C. Moreno, and W. E. Brown, Arch. OraEBiul., 11, 477 (1966).
Reaction between Triplet Benzophenone and Diphenylamine (31) J. D.Termirie and E. D. Eanes, Calcif. Tissue Res., I O , 171 (1972). (32) H. Furedi-Milhoier, 8. Purgaric, L. Brecevic, and N. Pavkovic, Ca/cif. 77ssue Res., 8, 142 (1971:l. (33) W. G.Robertson, &kif. Tissue Res., 11, 311 (1973). (34) J. IC. Bell, A. M Posner, and J. P. Quirk, J. Colloid Interface Sci., 42, 250
225 (35) B. Tezak, E. Matijevic, and K. Schuiz, J. Phys. Colloid Chem., 65, 1567 (1951). (36) W. F. Newman, T. Y. Toribara, and B. J. mu^^^^^ Arch. Biochem. Biophys., 98, 384 (1962). (37) R. A. Robinson and M. L. Watson, Ann. pi. Y. Acad. Sci., ( 1955).
n between Triplet Benzophenone and Diphenylamin
%me$H. Marshall Bell laboratories, Murray Hi//, New Jersey 07974 (Received January 30, 1974; Revised Manuscript ReceivedJune 13, 1974) ~ u ~ l i c 2 icosts ~ j o ~assisted by Bell Laboratories
ell-resolved esr spectra of the diphenylamino radical are detected upon the uv irradiation of benzene solutions of benzophenone and diphenylamine. The diphenylamino radicals are presume drogen atom abstraction by triplet benzophenone. Using naphthalene as a triplet quencher, the rate of this initial reaction is found to be 2.3 X lo9 M - l sec-l or nearly diffusion controlled. Because substantial overall reversible character is apparent during steady photolysis, while the initial reaction appears to be irreversible, a series of reactions is proposed in order to regenerate the starting materials.
I n ~ r ~ ~ ~ ~ c t i o ~ ~ Although the esr spectra of many related radicals have been until recently the spectrum of the diphenylamino radical (Ph2N.)4had not been clearly identified. Hoskins5 heated solutions of tetraphenylhydrazine (Ph2NNPh2), bait observed only diphenyl nitroxide and another spectrum w ichl he attributed to a hydrazyl radical. Das, et u L . , ~ made am extensive esr study of Ph2NNPh2 derived radicals but apparently did not detect Ph2N.. Pannell,7 although initially reporting Ph&, later realized he had observed only diphenyl nitroxide upon the photolysis of diphenylamine (Ph2NI-I) in tert- butyl peroxide. Finally Neugebauer and Fischer2 recorded the isotropic esr spectra of a series of diarylaniino radicals, and subsequently Neugebauer and Bamberger4 detected the Ph2N. spectrum during the photolysis of P'h2NNPh2 in benzene solution. Tetraarylhydrazines thermally dissociate into diarylamino radicals in solution, and they are slowly destroyed by disproportionation and polymerization.s The photolytic dissociation products of PhgNNPh2 yield spectra with maxima a t 450 and 920 nm.9-p2By flash photolyzing benzene solutions of Ph2NNPh2 at room temperature, Sbida and Kirag observed that both absorptions decay by secondorder kinetics with a rate constant estimated to be 2.5 X lo7M-I sec- l. Benzophenone (Ph,$O) is efficiently photoexcited to a highly reactive n--?r*triplet state (Ph2CO(T1))13J4which can disappear by vairious processes including chemical reaction.15 Naphthalene (CloHs), with a triplet energy level substantially lower than that of Ph2CO(T1), quenches PhzCO(Tl) at a diffiision-controlled rate and thereby measurably inhibits most chemical reactions involving PhzCO(T1).'"
Reactions between photoexcited ones and amines + e t al.20 Results have been recently reviewed by Co suggest efficient quenching of Ph&O(Tl) by amines facilitated by some initial degree of charge-transfer between PhZCO(T1) and amine.21-26. Accompanying this high quenching rate is a low quantum yield for photoreduction of PhzCO. The rate of Ph2CO(T1) quenching by Ph2NI-I in %propanol .is nearly diffusion controlled (k I^ 4.3 >( lo9 M - l ~ e c - l ) and , ~ ~PhzCO's photoreduction in 2-methyl-%propano1 and acetonitrile by PhzNH is slow, although producing a high percentage of 44N- p h ~ n y 1 a m ~ ~ ~ ) ~ b e n y l d i p ~ e n y l methanol and little 1,1,2,2-tetraphenyl-1,2-ethanediol. In benzene solution no photoproducts were detected,24 Reversible charge-transfer was invoked to account for the apparent high degree of reversibility in 2-methyl-2-propanol and acetonitrile. Davidson, et al., 2 5 confirmed the low yield of isolatable products from the photolysis of Ph&O and Ph2NE-I. By flash techniques they determined that the hydroxydiphenylmethyl radical (Ph&OH) was produced, and that a t low concentrations of Ph&O (5 X M ) and of aniline, otoluidine, or PhzNH (ea. MI Ph26:OI-I dec first-order mechanism. They post reacting with Ph2NH. Although Ph2N. was produced along with PEb2(3XI, that when benzene, 2-methyl-2-propano1, and acetonitrile solutions of Ph&O and aniline were flashed, only Ph&3W and anilino radicals, and no radical ioiis, were detected. The anilino radical decay was second order.
xperimental Section The esr spectrometer is a Varian %-band system using The Journal of Physical Chemistry. Val. 78, No. 22, 1974